The presence of calcium hydroxide (CH) can pose deteriorating effect on the durability of the cement from the inclusion of Eggshell powder (ESP) into the cement matrix. The incorporation of supplementary cementitious materials (SCM) such as Saw dust ash (SDA) could improve the properties of ESP-cement blends by eliminating some undesirable effects at the later age. This paper tries to explore the effect of possibility of replacing eggshell powder (ESP) cement blend with SDA and cement replacement on the properties such as consistence, setting times, volume expansion and strength gain. Saw dust was calcined at 600°C for 1 hour and sieved with 90µm sieve to obtain SDA. Portland limestone cement CEM II A-L was blended with ESP was replaced with SDA between 0 – 20 wt.% at 5 wt.% intervals and 0 -12.5 wt.% at 2.5 wt.% interval for physical properties and mortar compressive strength using 50 mm cubes with mixing ratio 1:3:5 (water, binder and sand) respectively. The chemical analysis of SDA revealed a high silica content (56.81 wt.%) with SiO2+Al2O3+Fe2O3 > 70% (72.2 wt.%), thus classified as Class F pozzolan according to ASTM C618 while ESP indicated a high lime content (48.5 wt.%) and considered a filler. Results indicated an increase in the consistence and setting time of the ternary blends as ESP was replaced with SDA owing to the unburnt carbon present in the SDA as well as clinker diminution. Likewise, an increase in the cement replacement led to an increase in water consistence and setting times. The retarded setting times of SDA-ESP cement blends could be attributed to increased water required due to SDA’s unburnt carbon whereas, ESP-cement blend produced accelerated setting times. A decrease in the volume expansion of the cement blends was observed as ESP was replaced with SDA which could be attributed to the decrease in the available lime while an increase in the volume expansion was also experienced as the cement replacement was increased from 0 – 20 wt.% at various SDA/SDA-ESP ratios from 0 – 0.8 except ratio of 1.0. The mortar compressive strength of cement blended with ESP and SDA experienced an increase as curing age was lengthened despite clinker diminution. This enhanced strength could be linked with SDA’s pozzolanic reactivity, provision of nucleation sites and formation of muscovite resulting in denser CSH with the optimal cement replacement observed at 5 wt.% with SDA/SDA-ESP ratio of 0.2 and 0.4 respectively.
Olubajo Olumide Olu,
Effect of Saw Dust Ash and Eggshell Powder on the Properties of Cement Blends, American Journal of Construction and Building Materials.
Vol. 4, No. 2,
2020, pp. 88-99.
Gowsika, D., Sarankokila, S., and Sargunan, K. (2014). Experimental investigation of egg shell powder as partial replacement with cement in concrete. International Journal of Engineering Trends and Technology (IJETT), 14 (2), 65-68.
Tiamiyu, I. A. (1997). Strength characteristics of cement-rice husk ash concrete. B. Eng Project, Department of Civil Engineering, Bayero University, Kano, pp. 52.
Shiathas C., Muntasser, T. Z., and Nwaubani, S. O. (2000). A comparative study of the properties and durability of binary and ternary cementitious systems. pg. 3.
Damloft, J. S., Lukasik, J., Herfort, D., Sorrentino, D., and Gartner, E. M. (2008). Sustainable development and climate change initiatives. Cement and Concrete Research, 38 (2), 115-127.
Matawal, D. S. (2005). Application of ashes as pozzolana in mortar and concrete production. 1st National Academy Conference 31,
Snelson, D., Wild, S., and O’Farrel, M. (2011). Setting times of Portland cement – metakaolin-fly ash blends. Taylor and Francis, 17, 55–62.
Dave, N., Misra, A. K., Srivastava, A., and Kaushik, S. K. (2016). Setting time and standard consistency of quaternary binders: The influence of cementitious material addition and mixing. International Journal of Sustainable Built Environment, 1-7.
Marthong, C. (2012). Sawdust ash (SDA) as partial replacement of cement. International Journal of Engineering Research and Applications (IJERA), 2 (4), 1980-1985.
Nivedhitha, M., and Sivaraja M., (2017) Experimental study on partial replacement of cement with coconut shell powder and egg shell powder. International Journal of Innovative Research in Science, Engineering and Technology, 6 (5), 8505-8511.
Praveen, K. R., Vijaya, S. R., and Jose, V. B. (2015). Experimental study on partial replacement of cement with eggshell powder. International Journal of Innovations in Engineering and Technology (IJIET), 2 (5), 334-341.
Dhanalakshmi, M., Sowmya, N. J., and Chandrashekar, A. (2015) A comparative study on egg shell concrete with partial replacement of cement by fly ash. International Journal of Engineering Research and Technology (IJERT). 4 (5), 1532-1539.
Amarnath, Y. (2014). Properties of concrete with eggshell powder as cement replacement. Indian Concrete Journal pg. 1-10.
Jayasankar, R., Mahindran, N., and Ilangovan, R. (2010). Studies on concrete using fly ash, rice husk ash and egg shell powder. International Journal of Civil and Structural Engineering, Integrated Publishing Services. ISSN 0976-4399, 1 (3), 362-372.
Al-Heaty, A. K. (2000). Controlling slump loss problems in ready mix high resistance concrete exposed to sever solutions”, MSc. Thesis, University of Technology.
Kumar, R. R., Mahendran, R., S., Nathan, S. G., Sathya, D. and Thamaraikannan K. (2017). An experimental study on concrete using coconut shell ash and egg shell powder. South Asian Journal of Engineering and Technology, 3 (7), 151-161.
Mastan, S. A., and Kumar, V. R. P. (2015). Experimental study on concrete by partial replacement of fine aggregate with fly ash and egg shell powder. International Journal and Magazine of Engineering, Technology, Management and Research: A Peer Reviewed Open Access International Journal. 2 (2), 214-220.
Karthick, J., Jeyanthi, R., and Petchiyamma, M. (2014). Experimental study on usage of egg shell as partial replacement for sand in concrete. International Journal of Advanced Research in Education Technology (IJARET) 1 (1) 7-10.
Mohamed, A. M., Dinesh K. M., Milan C. J., and Vani, G., (2016) Replacement of cement using eggshell powder SSRG International Journal of Civil Engineering (SSRG - IJCE) 3 (3), 1-2.
Ogork, E. N., and Ayuba, S. (2014). Influence of sawdust ash (SDA) as admixture in cement paste and concrete. International Journal of Innovative Science, Engineering and Technology IJISET, 1 (10), 736-743.
Batt, A. S., and Garg, A. (2017). Partial replacement of wood ash with ordinary Portland cement and foundry sand as fine aggregate. Journal of Civil Environ and Engineering, 7, 272. doi: 10.4172/2165-784X.1000272.
Chowdhury, S., Maniar, A., and Suganya, O. M. (2015). Strength development in concrete with wood ash blended cement and use of soft computing models to predict strength parameters. Journal of Advanced Research, 6 (6), 907–913.
Raheem, A. A., Olasunkanmi, B. S., and Folorunso, C. S. (2012). Saw dust ash as partial replacement for cement in concrete. Organization, Technology and Management in Construction and International Journal. 4 (2), 474-480.
Sanjay, C., and Rahul, B. (2016). Study on saw dust ash as partial replacement with cement. International Journal of Engineering Technology Science and Research (IJETSR) 3 (4), 126-130.
Obilade, I. O. (2014). Use of saw dust ash as partial replacement for cement in concrete. International Journal of Engineering Science Invention 3 (8), 36-40.
Malik, M. I., Jan, S. R., Peer, J. A., Nazir, S. A. and Mohammad, K. F. (2015). Partial replacement of cement by saw dust ash in concrete a sustainable approach. International Journal of Engineering Research and Development 11 (2), 48-53.
Shetty, M. (2005). Concrete technology: Theory and practice: S. Chand.
Morsy, M., and Shebl, S. S. (2007). Effect of silica fume and metakaolin pozzolana on the performance of blended cement pastes against fire. Ceramics Silikaty, 5 (1), 40-44.
Olubajo, O., Osha, O., El-Natafty, U., and Adamu, H. (2017). A study on Coal bottom ash and limestone effects on the hydration and physico-mechanical properties of ternary cement blends (Doctoral thesis). Abubakar Tafawa Balewa University, Bauchi, Nigeria.
ASTM C 187, (2010). Standard test method for normal consistency of hydraulic cement. Annual Book of ASTM Standards.
ASTM C 191 – 19 (2010). Standard test method for Time of Setting of hydraulic cement by Vicat Needle. Annual Book of ASTM Standards.
ASTM C151. (2000). Standard test method for autoclave expansion of Portland cement, Document Number: ASTM C151-00, ASTM International.
ASTM C 109 (2008). Standard test method for compressive strength of hydraulic cement mortars. Annual Book of ASTM Standards.
Bureau of Indian Standards. (1988). Methods of physical tests for hydraulic cement. Part 6: Determination of compressive strength of hydraulic cement (Other than masonry cement) (IS 4031: 1988). New Delhi: Bureau of Indian Standards.
ASTM C 618 (2008). Standard specification for coal fly ash and raw or calcined natural pozzolan for use in concrete. Annual Book of ASTM Standards
Kaya, A. (2010, September). A study on blended bottom ash cements (Master’s thesis). Retrieved from http://etd.lib.metu.edu.tr/upload/12612504/index.pdf.
Olubajo, O. O., and Osha, O. A. (2013). Influence of bottom ash and limestone powder on the properties of ternary cement and mortar. International Journal of Engineering Research and Technology 2 (7), 1201-1212 Available on website link: http://www.ijert.org.
Bonavetti, V., Rahhal, V., and Irassar, E. (2001). Studies on the carboaluminate formation in limestone filler-blended cements. Cement and Concrete Research, 31 (6), 853–859. doi: 10.1016/s0008-8846(01)00491-4
Soroka, I. and Setter, N. (1977). The effect of fillers on strength of cement mortars. Cement and Concrete Research, 7 (4), 449-456.
Péra, J., Husson, S., and Guilhot, B. (1999). Influence of finely ground limestone on cement hydration. Cement and Concrete Composites, 21 (2), 99-105.
Ramachandran, V. S. and Zhang C. (1986). Thermal analysis of the 3CaO• Al2O3-CaSO4• 2H2O-CaCO3-H2O system. Thermochimica acta, 106, 273-282.
Lothenbach, B., Le Saout, G., Gallucci, E., and Scrivener, K. (2008). Influence of limestone on the hydration of Portland cements. Cement and Concrete Research, 38 (6), 848-860.
De Weerdt, K., Kjellsen, K. O., Sellevold, E. and Justnes, H. (2011). Synergy between fly ash and limestone powder in ternary cements. Cement and Concrete Composites, 33 (1), 30-38.
Barker, A., and Cory, H. P. (1991). The early hydration of limestone-filled cements. In Blended cements in construction. Papers presented at the International conference, University of Sheffield, UK, 9-12 September 1991.
Kakali, G., Tsivilis, S., Aggeli, E., and Bati, M. (2000). Hydration products of C3A, C3S and Portland cement in the presence of CaCO3. Cement and Concrete Research, 30 (7), 1073-1077.
Olubajo O. O., Abubakar J., and Osha O. A. (2020) The effect of eggshell ash and locust bean pod ash on the compressive strength of ternary cement. Path of Science, 6 (3), 4001-4016. Available on website link: http://www.pos.org
Deng, M. (1992). Mechanism of MgO expansion in cement. Cement and Concrete 22, 1-5.
Ikumapayi, C. M. (2017). Crystal and microstructure analysis of pozzolanic properties of bamboo leaf ash and locust beans pod ash blended cement concrete. Journal of Applied Sciences and Environmental Management, 20 (4), 943. doi: 10.4314/jasem.v20i4.6.
Spelta, J. S. de O., and Galdino, A. G. de S. (2018). Bioceramic composite: hen’s eggshell characterization and main applications. Revista Ifes Ciência, 4 (1), 9–20. doi: 10.36524/ric.v4i1.323.
Ojewumi, M., Ayomide, A., Obanla, O., Awolu, O., and Ojewumi, E. (2016). Pozzolanic properties of waste agricultural biomass – African locust bean pod waste. World Journal of Environmental Biosciences, 6 (3), 1–7.
Venkateswara, R., Kontham, G., Venkata, R., and Chundupalli, S. (2011). Effect of potassium chloride (KCl) on ordinary Portland cement (OPC) concrete. Research Journal of Chemical Sciences, 1 (2), 103–107.
Tang, R. A. (2010, November). Compressive strength of normal strength concrete (NSC) using British Standard, Euro code and non-destructive test approaches (Bachelor’s thesis). Retrieved from http://umpir.ump.edu.my/id/eprint/3297/1/TANG_JIAN _AN.PDF.
Mangi, S. A., Jamaluddin, N., Ibrahim, W. M. H., Mohamad, N., and Sohu S. (2017). Utilization of sawdust ash as cement replacement for the concrete production: A review. Engineering Science and Technology International Research Journal, 1 (3), 11-15.